This preview shows pages 1–3. Sign up to view the full content.
This preview has intentionally blurred sections. Sign up to view the full version.
View Full Document
Unformatted text preview: Exercise 15.1 Subject: Estimation of adsorbent characteristics. Given: Porous particles of activated alumina. BET area = 310 m 2 /g = S g . Particle porosity = 0.48 = p . Particle density = 1.30 g/cm 3 = p . Assumptions: Straight pores of circular crosssection with uniform diameter. Find: (a) V p = specific pore volume in cm 3 /g. (b) s = true solid density, g/cm 3 . (c) d p = average pore diameter, angstoms. Analysis: (a) From Eq. (153), V p = p / p = 0.48/1.30 = 0.369 cm 3 /g (b) From a rearrangement of Eq. (155), s = p /(1  p ) = 1.30/(1  0.48) = 2.50 g/cm 3 (c) From a rearrangement of Eq. (152), d p = 4 p / S g g = 4(0.48)/[310 x 10 4 (1.30)] = 4.76 x 107 cm or 47.6 angstroms. Exercise 15.2 Subject: Estimation of surface area of two forms of molecular sieves. Given: Form A with V p = 0.18 cm 3 /g and average d p = 5 angstroms. Form B with V p = 0.38 cm 3 /g and average d p = 2.0 microns. Assumptions: Straight pores of circular crosssection with uniform diameter. Find: Surface area, S g , of each form. Analysis: By substitution of Eq. (153) into (152), S g = 4 V g / d p (1) Form A: From Eq. (1), S g = 4(0.18)/(5 x 108 ) = 14.4 x 10 6 cm 2 /g or 1,440 m 2 /g Form B: From Eq. (1), S g = 4(0.38)/(2 x 104 ) = 7,600 cm 2 /g or 0.760 m 2 /g This is a very large difference in surface area. Exercise 15.3 Subject: Consistency of the characteristics of a smallpore silica gel. Given: Smallpore silica gel. Pore diameter = 24 angstroms = d p . Particle porosity = 0.47 = p . Particle density = 1.09 g/cm 3 = p . Specific surface area = 800 m 2 /g = S g . Assumption: Straight pores of circular crosssection with uniform diameter. Find: (a) Reasonableness of the above values. (b) Fraction of a monolayer adsorbed if the adsorption capacity for water vapor at 25 o C and 6 mmHg partial pressure is 18% by weight. Analysis: (a) From Eq. (152), based on the above assumption, S g = 4 p / d p g = 4(0.47)/[(1.09 x 10 6 )(24 x 1010 )] = 719 m 2 /g This is reasonable compared to the given value of 800 m 2 /g. The true density of silica gel, assuming it is SiO 2 , depends on its crystalline form. From a handbook, the density is from 2.20 to 2.65 g/cm 3 , with 3 of 4 forms from 2.20 to 2.26 g/cm 3 . Therefore, using a value of s = 2.20 g/cm 3 with Eq. (155), p = 1  p / s = 1  1.09/2.20 = 0.505 . This is reasonable compared to the given value of 0.47 . (b) From the problem statement, it is not clear whether the 18 wt% refers to a dry basis or a wet basis, so consider both possibilities. Dry basis: Adsorb 0.18 grams water per 1.0 gram of waterfree silica gel. Therefore, for 1.0 gram of dry silica gel, the surface area for adsorption = 800 m 2 ....
View
Full
Document
This note was uploaded on 04/27/2011 for the course CHEM 101 taught by Professor Suh during the Spring '11 term at University of Toronto Toronto.
 Spring '11
 suh

Click to edit the document details